| ||Format||Pages||Price|| |
|5||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$62.00||  ADD TO CART|
Significance and Use
5.1 Relative density (specific gravity) is the ratio of mass of an aggregate to the mass of a volume of water equal to the volume of the aggregate particles – also referred to as the absolute volume of the aggregate. It is also expressed as the ratio of the density of the aggregate particles to the density of water. Distinction is made between the density of aggregate particles and the bulk density of aggregates as determined by Test Method C29/C29M, which includes the volume of voids between the particles of aggregates.
5.2 Relative density is used to calculate the volume occupied by the aggregate in various mixtures containing aggregate, including hydraulic cement concrete, bituminous concrete, and other mixtures that are proportioned or analyzed on an absolute volume basis. Relative density (specific gravity) is also used in the computation of voids in aggregate in Test Method C29/C29M. Relative density (specific gravity) (SSD) is used if the aggregate is in a saturated-surface-dry condition, that is, if its absorption has been satisfied. Alternatively, the relative density (specific gravity) (OD) is used for computations when the aggregate is dry or assumed to be dry.
5.3 Apparent relative density (specific gravity) pertain to the solid material making up the constituent particles not including the pore space within the particles that is accessible to water.
5.4 Absorption values are used to calculate the change in the mass of an aggregate due to water absorbed in the pore spaces within the constituent particles, compared to the dry condition, when it is deemed that the aggregate has been in contact with water long enough to satisfy most of the absorption potential. The laboratory standard for absorption is that obtained after submerging dry aggregate for a prescribed period of time. Aggregates mined from below the water table commonly have a moisture content greater than the absorption determined by this test method, if used without opportunity to dry prior to use. Conversely, some aggregates that have not been continuously maintained in a moist condition until used are likely to contain an amount of absorbed moisture less than the 24-h soaked condition. For an aggregate that has been in contact with water and that has free moisture on the particle surfaces, the percentage of free moisture is determined by deducting the absorption from the total moisture content determined by Test Method .
5.5 The general procedures described in this test method are suitable for determining the absorption of aggregates that have had conditioning other than the 24-h soak, such as boiling water or vacuum saturation. The values obtained for absorption by other test methods will be different than the values obtained by the prescribed soaking, as will the relative density (specific gravity) (SSD).
1.1 This test method covers the determination of relative density (specific gravity) and the absorption of coarse aggregates. The relative density (specific gravity), a dimensionless quantity, is expressed as oven-dry (OD), saturated-surface-dry (SSD), or as apparent relative density (apparent specific gravity). The OD relative density is determined after drying the aggregate. The SSD relative density and absorption are determined after soaking the aggregate in water for a prescribed duration.
1.2 This test method is not intended to be used with lightweight aggregates that comply with Specification Group I aggregates.
1.3 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.4 The text of this test method references notes and footnotes that provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of this test method.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C29/C29M Test Method for Bulk Density (Unit Weight) and Voids in Aggregate
C125 Terminology Relating to Concrete and Concrete Aggregates
C128 Test Method for Density, Relative Density (Specific Gravity), and Absorption of Fine Aggregate
C136 Test Method for Sieve Analysis of Fine and Coarse Aggregates
C330 Specification for Lightweight Aggregates for Structural Concrete
C332 Specification for Lightweight Aggregates for Insulating Concrete
C566 Test Method for Total Evaporable Moisture Content of Aggregate by Drying
C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials
C702 Practice for Reducing Samples of Aggregate to Testing Size
D75 Practice for Sampling Aggregates
D448 Classification for Sizes of Aggregate for Road and Bridge Construction
E11 Specification for Woven Wire Test Sieve Cloth and Test Sieves
ICS Number Code 91.100.30 (Concrete and concrete products)
UNSPSC Code 30111800(Aggregates)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C127-15, Standard Test Method for Relative Density (Specific Gravity) and Absorption of Coarse Aggregate, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top